#------------------------------------------------------------------------------
#$Date: 2024-04-25 17:59:02 +0300 (Thu, 25 Apr 2024) $
#$Revision: 291351 $
#$URL: file:///home/coder/svn-repositories/cod/cif/9/00/27/9002732.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the American Mineralogist Crystal Structure Database,
# http://rruff.geo.arizona.edu/AMS/amcsd.php
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_9002732
loop_
_publ_author_name
'Effenberger, H.'
'Paar, W. H.'
'Topa, D.'
'Criddle, A. J.'
'Fleck, M.'
_publ_section_title
;
 The new mineral baumstarkite and a structural reinvestigation of
 aramayoite and miargyrite
;
_journal_name_full               'American Mineralogist'
_journal_page_first              753
_journal_page_last               764
_journal_volume                  87
_journal_year                    2002
_chemical_formula_sum            'Ag Bi0.334 S2 Sb0.666'
_chemical_name_mineral           Aramayoite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                100.32
_cell_angle_beta                 104.07
_cell_angle_gamma                90.18
_cell_length_a                   7.813
_cell_length_b                   8.268
_cell_length_c                   8.880
_cell_formula_units_Z            6
_cell_volume                     546.763
_database_code_amcsd             0002821
_exptl_crystal_density_diffrn    5.884
_cod_original_formula_sum        'Ag (Sb.666 Bi.334) S2'
_cod_database_code               9002732
loop_
_space_group_symop_operation_xyz
x,y,z
-x,-y,-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
Ag1 0.11503 0.42287 0.14742 1.00000
Ag2 0.30433 0.07450 0.84722 1.00000
Ag3 0.00914 0.74334 0.49858 1.00000
Sb1 0.64238 0.41787 0.16524 0.93700
Bi1 0.64238 0.41787 0.16524 0.06300
Sb2 0.16700 0.91841 0.16979 0.96300
Bi2 0.16700 0.91841 0.16979 0.03700
Bi3 0.49374 0.24679 0.49421 0.90300
Sb3 0.49374 0.24679 0.49421 0.09700
S1 0.85745 0.20464 0.20003 1.00000
S2 0.38019 0.25024 0.16822 1.00000
S3 0.73044 0.52180 0.46193 1.00000
S4 -0.02532 0.69719 0.19690 1.00000
S5 0.43666 0.76178 0.18244 1.00000
S6 0.23938 0.02194 0.46306 1.00000
loop_
_cod_related_entry_id
_cod_related_entry_database
_cod_related_entry_code
1 AMCSD 0002821
